THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH


 Frederick Morton
 9 months ago
 Views:
Transcription
1 THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK SUMMARY Delamination is usually associated with throughthickness failure, but in fact can have a major effect on inplane strength of notched and unnotched laminates. This paper considers tensile strength of quasiisotropic laminates and results from scaled tests to show how delamination is critical in damage development and ultimate failure. Keywords: Delamination, Tensile strength, Notches, Hole size effect, Scaling INTRODUCTION Delamination is widely recognised as the Achilles heel of composite structures. A lot of effort has gone into researching delamination due to throughthickness stresses arising at features such as ply drops and free edges [e.g. 1, 2]. However, it is less widely appreciated that delamination also has a crucial role in determining inplane strength, often leading to premature initiation of failure. Failure of composites is driven by the energy released as they are unloaded. This can occur in two ways: by fibre failure, or by delamination and matrix cracks joining up to produce a fracture surface without the need to break fibres. The latter mechanism is illustrated in Fig. 1 which shows schematically a (45/45)s laminate that has failed in tension by pullout without any fibre failure. Similar phenomena can also affect failure in other layups. In this paper the role of delamination in unnotched and notched tensile strength of quasiisotropic laminates is considered, and it is shown to have a large effect on the failure mechanism and stresses. Figure 1: Schematic of pullout failure of (45/45)s laminate with no fibre fracture
2 UNNOTCHED TENSILE STRENGTH A series of tests were carried out on quasiisotropic IM7/8552 carbonepoxy laminates with layup (45 m /9 m /45 m / m ) ns ) [3]. With m=1, n was varied from 1 to 4, giving laminates from 1 to 4 mm thick with dispersed plies. Keeping n=1 and increasing m from 2 to 8 gave laminates from 2 to 8 mm thick with a single set of repeating plies with different ply block thicknesses. The stacking sequence was selected to minimise the risk of edge delamination. Strain energy release rate calculations were performed using a finite element model of a slice perpendicular to the loading direction [4]. This analysis method was applied to all 12 possible symmetric quasiisotropic stacking sequences with 8 plies, and the one with the highest edge delamination strain of those with a 45º surface ply was selected. The smallest specimens were 1 mm thick, 8 mm wide, with a gauge section of 3 mm, and bonded glassepoxy end tabs. Thicker specimens had the inplane dimensions increased in proportion to the thickness so that they were fully scaled. The expected failure stress was calculated using laminated plate theory with the properties shown in Table 1, and the unidirectional tensile strength of 286 MPa measured with a small tapered thickness specimen with chamfered plies [3]. This gave a quasiisotropic strength of 177 MPa. Table 1: Ply properties for IM7/8552 º modulus E GPa 9º modulus E GPa Shear modulus G GPa Poisson s ratio ν Experimental results are summarized in Table 2, and plotted in Fig. 2. There are large differences between different layups and none of them reached the expected strength. This is due to initiation of delamination at the free edge. This could clearly be seen in the 2 mm thick specimens with blocked plies, Fig. 3. Subsequently the fibres also break, but the initial failure is controlled by delamination. When more plies are blocked together, delamination occurs at even lower stresses and becomes the main failure mechanism, stepping down through the plies until complete separation occurs at the 45/ interface prior to fibre failure. The same mechanism is believed to control the strength of the dispersed ply specimens, with initiation of free edge delamination leading straight away to fibre failure. In this case the strength actually increases with thickness, because the multiple sublaminates inhibit the free edge delamination initiating from the surface plies. Laminated plate theory gives the same expected strength for all these cases. The large variation in strengths which are all below this value are due to the differences in delamination behaviour of the different laminates.
3 Table 2: Unnotched failure stresses of quasiisotropic IM7/8552 laminates Blocked plies, m Repeated sublaminates, n Thickness (mm) Layup Failure stress (MPa) (45/9/45/) 4S (45/9/45/) 2S (45/9/45/) S (45 2 /9 2 /45 2 / 2 ) S (45 4 /9 4 /45 4 / 4 ) S (45 8 /9 8 /45 8 / 8 ) S 321 Tensile strength (MPa) Dispersed plies Blocked plies Thickness (mm) Expected Dispersed Blocked plies plies Figure 2: Effect of thickness and ply blocking on unnotched tensile strength Line of fibre fracture delamination matrix crack a b c Figure 3: Photographs and schematic of failure in (45 2 /9 2 /45 2 / 2 ) S specimens
4 NOTCHED TENSILE STRENGTH Delamination and the stress at which it occurs relative to fibre failure is similarly important in notched strength. For example in open hole tension of (45/9/45/)s laminates with thick ply blocks delamination and pullout can occur leaving two ligaments of unidirectional material as shown in Fig. 4 [5]. Figure 4: Schematic of pullout in notched quasiisotropic laminate This is shown on a series of scaled specimens of the same material and stacking sequence as the previous unnotched ones. Specimens with a centrally located circular hole were tested in tension with constant width to hole diameter (W/D) and length to hole diameter (L/D) ratios, as shown in Fig. 5. Gripping region Gauge section W/D = 5 D L/D = 2 Figure 5: Open hole specimen geometry Results of 4 mm thick specimens with blocked plies are plotted in Fig. 6, with a log scale to better cover the wide range of hole sizes from 1.6 to 5.4 mm. All failures were controlled by delamination, and there was a considerable variation in strength with specimen size. There is a clear trend with the strengths transitioning between a lower and a higher asymptote as the hole size increases. Triangular delaminations similar to those observed in the unnotched specimens formed at the intersection of the surface 45 ply and the free edges, and grew gradually across the width between the hole and straight edge in both directions. It appears that the point at which these span the complete width of the specimen corresponds to the point when the delamination is able
5 to step down through the remaining plies to the 45/ interface and propagate along the whole length. Comparing these results with the previous unnotched tests on specimens 32 mm wide with the same layup and similar damage development shows that the unnotched case fits well as an asymptote at large hole sizes, Fig. 6. The size of the triangular delaminations at the free edges is related to the ply block thickness. It might therefore be expected that if the specimen was very narrow, these would be able to join up across the complete width more easily, leading to earlier onset of full delamination. To test this hypothesis, unnotched specimens of the same layup with a width of only 4 mm were tested in tension. These delaminated in a similar way, but at an average stress of only 266 MPa. This is also shown as a line on Fig. 6, and fits well as a lower asymptote. Failure stress (MPa) D (mm) Notched Unnotched w=32mm Unnotched w=4mm Fit Figure 6: Effect of hole size on delamination stress of (45 4 /9 4 /45 4 / 4 ) s ) laminates The notched strength of these specimens is therefore controlled by how easily delamination can occur. This depends on two main factors: the absolute ply block thickness, which controls the total amount of energy available to drive delamination and the ratio of ply block thickness to distance from the free edge which affects how easily it can propagate across the width. If the specimens are normalised in such a way as to account for the different propensity to delaminate and plotted against ligament width rather than hole size, we can account for a whole range of different cases on a single plot. This is done using equation (1) to normalise the failure stress by the amount of available energy based on the ply block thickness T ply compared with the baseline.5 mm of the specimens shown in Fig. 6. σ = σ T ply.5 (1) Results are plotted in Fig. 7 for open hole specimens with thinner and thicker ply blocks, and also for another set of tests on the same material where a W/D ratio of 1 was used as well as 5. All these specimens failed by delamination. A finite width
6 correction was applied to the latter results to ensure direct comparability. The results all fit reasonably well the trend shown earlier, confirming the parameters controlling tensile strength of open hole specimens failing by delamination. Normalised failure stress (MPa), Eq. (1) Ligament width/tply m=4, Tply=.5mm Unnotched w=32mm Unnotched w=4mm Fit m=8, Tply=1mm m=2, Tply=.25mm m=2, varying w/d Figure 7: Effect of ply block thickness and ligament width on delamination of (45 m /9 m /45 m / m ) s ) laminates With thinner, dispersed plies this same mechanism causes subcritical damage development, leading to blunting of the notch before reaching the delamination stress, hence increasing the fibre dominated tensile strength. Open hole tests with the same 4 mm thickness, but with dispersed plies all showed fibre failure, and a decreasing strength with increasing hole size. This is shown in Fig. 8, contrasting with the increasing strength with hole size found for the same thickness specimens with plies blocked together. Failure stress (MPa) D (mm) Dispersed plies, fibre failure Blocked plies, delamination Figure 8: Open hole tensile strength of 4 mm thick quasiisotropic specimens
7 Although the dispersed ply specimens did not fail by complete delamination, there was still some localised delamination at the hole edge starting at matrix cracks. Initially the size of these delaminations was of the order of the ply thickness, but later they extended and joined up, stepping through the thickness locally. This behaviour adjacent to the hole is similar to that observed globally in the unnotched specimens and in the notched specimens failing by overall delamination. Splitting in the plies also occurred, blunting the notch, and allowing the stress to reach a higher value than the unnotched strength divided by the stress concentration factor. As the hole size to ply block thickness ratio increases, it becomes more difficult for the delaminations at the hole edge to join up and for splitting to occur, and so this same parameter is also relevant for the fibre failure cases, causing a reduction in strength with increasing size as damage is inhibited. This is illustrated schematically in Fig. 9, showing just the 45 and 45 cracks. For a small hole, the delaminations associated with the transverse cracks almost overlap, facilitating damage linking up through the thickness and propagating. Figure 9: Delaminations from ply cracks can join up more easily for small holes The relation between delamination and fibre failure can be better understood by plotting the results controlled by delamination in Fig. 6 and those controlled by fibre failure in Fig. 8 on the same graph, but with the stresses corrected to account for the propensity to delaminate. The normalisation is based on the same principle as equation (1), extended to account for the effect of multiple ply blocks on the amount of energy available to drive delamination of the surface 45 plies where failure initiates. Full details can be found in [5]. Fig. 1 shows that the normalised stresses of the thin dispersed ply specimens are well below the expected delamination stress, explaining why they all fail by fibre fracture. Tests have also been conducted on 4 mm thick specimens with two repeating sublaminates with.25 mm ply blocks, intermediate between the ones with.5 mm ply blocks that delaminated, and those with single.125 mm plies that gave fibre failures. These are also plotted on Fig. 1. The larger three sizes with.25 mm ply blocks all fall well below the trend for delamination, and fibre failures were indeed observed in
8 these cases. On the other hand the two smallest specimens failed by delamination, consistent with the fit to the blocked ply m=4, n=1 data, as discussed before. A transition in failure mode occurs when fibre failure is reached before delamination. Normalised failure stress (MPa), Eq. (3) Transition in failure mode, m=2, n= D/Tply m=4, n=1 Fit m=1, n=4 m=2, n=2 Fibre failure Others delamination 4 Figure 1: Failure mode and hole size effect for 4 mm (45 m /9 m /45 m / m ) ns ) laminates It is also striking to see the different hole size effects for different ply block thicknesses, which can also be explained in terms of the role of delamination. With thick ply blocks delamination propagates right across the specimen, especially for small hole sizes with narrow ligaments. The delamination becomes the predominant failure mechanism, and gives rise to an increase in strength with hole size when the ratio of W/D is kept constant as it is harder for the delamination to propagate across the wider ligaments. With thin ply blocks the fibre failure stress is reached well before delamination initiating at the hole edge can propagate across the width, and so fibre failure occurs. It is still more difficult for delamination to propagate as the hole size increases, but this now means that the beneficial effect of delamination and splitting on blunting the notch is reduced. The strength reduces with increasing hole diameter, giving rise to the conventional hole size effect. With.25 mm ply blocks the failure mechanism is at the transition between delamination and fibre failure. In specimens with small holes the delamination propagates across the complete width, constituting failure, whereas for the larger ones fibre failure occurs first. The competing failure mechanisms result in an almost constant strength between 1.6 and 12.7 mm holes. CONCLUSIONS Delamination has a major effect on unnotched and notched tensile strength of quasiisotropic carbon fibre/epoxy laminates. Unnotched specimens with different ply block thicknesses and numbers of sublaminates showed differences in strength of nearly a
9 factor of three, with failure initiating by delamination at the free edge, and none of the specimens reaching the strength expected from laminated plate theory. Open hole tension specimens also fail by delamination for thick ply blocks, especially when the ratio of ply thickness to ligament width is large. Specimens with dispersed thin plies fail by fibre fracture before reaching the stress necessary to delaminate across the width. Delamination is still important in controlling splitting, and the associated reduction in the stress concentration factor. Increasing hole size may cause a decrease, increase or neutral effect on tensile strength for different ply block thicknesses depending on the relative propensity to delaminate. References 1. Wisnom MR, Dixon R, Hill G. Delamination in asymmetrically tapered composites loaded in tension, Composite Structures 1996: 35: O Brien TK. Mixedmode strain energy release rate effects on delamination of composites, effects and defects of composite materials, ASTM STP 836, American Society for Testing and Materials 1984: Wisnom MR, Khan B and Hallet SR. Size effects in unnotched tensile strength of unidirectional and quasiisotropic carbon/epoxy composites, Composite Structures 28: 84: Hallett SR, Jiang W, Khan B and Wisnom MR. Modelling the interaction between matrix cracks and delamination damage in scaled quasiisotropic specimens. Composites Science and Technology 28: 68: Wisnom MR and Hallett SR. The role of delamination in strength failure mechanism and hole size effect in open hole tensile tests, Composites Part A 29: 4:
University of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationThe Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/ Laminate in Tension, Compression and Bending
The Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/3506 Laminate in Tension, Compression and Bending Paul J. Callus Air Vehicles Division Defence Science and
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationDiscrete ply modelling of open hole tensile tests
Discrete ply modelling of open hole tensile tests Victor Achard, Christophe Bouvet, Bruno Castanié, Clément Chirol To cite this version: Victor Achard, Christophe Bouvet, Bruno Castanié, Clément Chirol.
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationApplication of a nonlocal failure criterion to a crack in heterogeneous media S. Bavaglia*, S.E. Mikhailov*
Application of a nonlocal failure criterion to a crack in heterogeneous media S. Bavaglia*, S.E. Mikhailov* University of Perugia, Italy Email: mic@unipg.it ^Wessex Institute of Technology, Ashurst Lodge,
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationLAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES. Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp.
LAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp. 12611266 INTRODUCTION Michael D. Seale and Barry T. Smith Departments
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationNumerical modelling of contact for low velocity impact damage in composite laminates J. Bonini, F. Collombet, J.L. Lataillade
Numerical modelling of contact for low velocity impact damage in composite laminates J. Bonini, F. Collombet, J.L. Lataillade Esplanade des Arts et Metiers, INTRODUCTION A low velocity impact on a composite
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 6 Fracture Toughness Testing and Residual
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationProgram: Recent Trends
The SNL/MSU/DOE Fatigue Program: Recent Trends John Mandell Montana State University 2012 SNL Blade Workshop May 30  June 1, 2012 Outline Overview of MSU Fatigue Program on Wind Blade Materials: Testing
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationDelamination in fractured laminated glass
Delamination in fractured laminated glass Caroline BUTCHART*, Mauro OVEREND a * Department of Engineering, University of Cambridge Trumpington Street, Cambridge, CB2 1PZ, UK cvb25@cam.ac.uk a Department
More informationDynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites
Engineering Fracture Mechanics 7 (5) 53 558 www.elsevier.com/locate/engfracmech Dynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites Sylvanus
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationIntroduction to scaling issues of damage and fracture in wind turbine blades
Introduction to scaling issues of damage and fracture in wind turbine blades Bent F. Sørensen Composites and Materials Mechanics Section Department of Wind Energy Technical University of Denmark Risø Campus,
More informationDELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE
DELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE F. LACHAUD 1,2, R. PIQUET 2, L. MICHEL 1 2 LMT, IUT de énie Mécanique, 50, Chemin des Maraîchers, 31077 TOULOUSE
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationMultiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading
Multiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading Robert Crouch 1, Caglar Oskay 1, and Stephen Clay 2 1 Department of Civil and Environmental Engineering, Vanderbilt University,
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationVIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS. Ana Andreia Pinheiro Durão Branco. Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho
VIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS Ana Andreia Pinheiro Durão Branco Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho Mestrado Integrado em Engenharia Mecânica July 17, 2015
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationElasticPlastic Fracture Mechanics. Professor S. Suresh
ElasticPlastic Fracture Mechanics Professor S. Suresh Elastic Plastic Fracture Previously, we have analyzed problems in which the plastic zone was small compared to the specimen dimensions (small scale
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationFinite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation
Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 Finite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation M. C. Song 1, B.V. Sankar 1, G. Subhash 1,
More informationOut life 30 days at 70 F (21 C) Shelf life 6 months at 40 F (4 C) 12 months at 0 F (18 C)
4708 250300 F (120150 C) High T g Epoxy Resin System Typical applications General aviation Aerospace Industrial Sporting goods Out life 30 days at 70 F (21 C) Shelf life 6 months at 40 F (4 C) 12 months
More informationNONDESTRUCTIVE EVALUATION METHODS FOR COMPOSITE PILES
NONDESTRUCTIVE EVALUATION METHODS FOR COMPOSITE PILES John F. Davila Graduate Research Assistant 2006 URIUPRM SUMMER INTERNSHIP RESEARCH PROGRAM Kingstown, RI July 29 of 2006 PRESENTATION OUTLINE Introduction
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationConcrete Technology Prof. B. Bhattacharjee Department of Civil Engineering Indian Institute of Technology, Delhi
Concrete Technology Prof. B. Bhattacharjee Department of Civil Engineering Indian Institute of Technology, Delhi Lecture  25 Strength of Concrete: Factors Affecting Test Results Welcome to module 6, lecture
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationSolid Mechanics Homework Answers
Name: Date: Solid Mechanics Homework nswers Please show all of your work, including which equations you are using, and circle your final answer. Be sure to include the units in your answers. 1. The yield
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationCombined Acoustic Emission and Thermographic Testing of Fibre Composites
19 th World Conference on NonDestructive Testing 2016 Combined Acoustic Emission and Thermographic Testing of Fibre Composites Matthias GOLDAMMER 1, Markus G. R. SAUSE 2, Detlef RIEGER 1 1 Siemens AG
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationA Method for Calculating Strain Energy Release Rates in Preliminary Design of Composite Skin/Stringer Debonding Under MultiAxial Loading
NASA/TM199909365 ARLTR01 A Method for Calculating Strain Energy Release Rates in Preliminary Design of Composite Skin/Stringer Debonding Under MultiAxial Loading Ronald Krueger National Research Council
More information